0 downloads
0 Views
74KB Size

Ind. Eng. Chem. Res. 2001, 40, 3775-3780

3775

SEPARATIONS Adsorption Isotherms of Benzoic Acid onto Activated Carbon and Breakthrough Curves in Fixed-Bed Columns Jia-Ming Chern* and Yi-Wen Chien Department of Chemical Engineering, Tatung University, 40 Chungshan North Road, 3rd Section, Taipei 10451, Taiwan

The adsorption isotherms of benzoic acid onto granular activated carbon at varying solution temperatures (25-55 °C) and pHs (2-8) from aqueous solution were experimentally determined by batch tests. The To´th model was found to fit all of the experimental data well. A series of column tests were performed to determine the breakthrough curves with varying bed depths (3-6 cm) and water flow rates (21.6-86.4 cm3/h). The results show that the half breakthrough time increases proportionally with increasing bed depth but decreases inverse proportionally with increasing velocity. The constant-pattern wave approach using the Freundlich isotherm model fits the experimental breakthrough curves quite successfully. A correlation was proposed to predict the volumetric mass-transfer coefficient in the liquid phase. Introduction Benzoic acid (BA) is widely used as a preservative or reaction intermediate and therefore often presents in domestic as well as industrial wastewaters. Because of its harmful effects, wastewaters containing BA must be treated before discharging to receive water bodies. Popular treatment processes include biological degradation,1-3 chemical oxidation,4,5 and adsorption.6-9 Among many adsorbents, granular activated carbon (GAC) is usually used in fixed-bed adsorption processes to remove organic pollutants such as BA. To properly design and operate fix-bed adsorption processes, the adsorption isotherm and the fix-bed dynamics, that is, the pollutant breakthrough curves, must be known. Various mass-transfer models10-15 were used to predict the breakthrough curves. To predict the breakthrough curve with a sophisticated mass-transfer model, one needs many parameters that must be determined by independent batch kinetic study or estimated by suitable correlations.11,14,15 Although a simplified method using one lumped parameter was developed by Wolborska and Pustelnik12 to predict the breakthrough times of fixed-bed adsorption processes, it can be applied for predicting the breakthrough curve in low concentration ranges with a linear adsorption isotherm only. If we want to predict the whole breakthrough curve, we need a model sophisticated enough to describe the main system features but simple enough to allow for analysis. A simple yet powerful tool that can be used to predict the breakthrough curves of fixed-bed adsorption processes without tedious calculations is the nonlinear wave propagation theory.16 In the prediction of the * To whom correspondence should be addressed. E-mail: [email protected] Tel: 886-2-25925252 ext 3487. Fax: 886-2-25861939.

breakthrough curves using the wave propagation theory, an infinite mass-transfer rate must be assumed to fulfill the local equilibrium conditions.17-19 Unfortunately, this assumption is not always met for fixed beds operated at high flow rates. Therefore, this study adopts the constant-pattern concept of the wave propagation theory along with the constant driving-force model to predict the breakthrough curves of carbon beds for BA removal. The effects of the flow rate and bed depth on the breakthrough curves will be investigated. The adsorption isotherms at varying solution temperatures and pHs will also be measured, and suitable model equations will be tried to fit the experimental data. Theory Consider a fixed-bed adsorber packed randomly with adsorbent particles that are fresh or just regenerated, and an aqueous solution containing an organic pollutant is fed to the top of the bed at a constant flow rate. The governing equation for predicting the fixed-bed dynamics is

∂q ∂C ∂C + u0 +F )0 ∂t ∂z ∂t

(1)

where F is the carbon bed density, F the void fraction of the bed, u0 the interstitial velocity of the carrier fluid, t the operating time, and z the distance from the inlet of the mobile phase and C and q are the pollutant concentrations in the mobile and stationary phases, respectively. Equation 1 is basically the unsteady-state mass balance of the adsorbate. The assumptions associated with eq 1 are as follows: (i) No chemical reactions occur in the column. (ii) Only mass transfer by convection is significant. (iii) Radial and axial dispersions are negligible. (iv) The flow pattern is ideal plug flow.

10.1021/ie010175x CCC: $20.00 © 2001 American Chemical Society Published on Web 07/21/2001

3776

Ind. Eng. Chem. Res., Vol. 40, No. 17, 2001

(v) The temperature in the column is uniform and invariant with time. (vi) The flow rate is constant and invariant with the column position. The adsorption rate of the pollutant can be described by the linear driving force model in terms of the overall liquid-phase mass-transfer coefficient:20

F

∂q ) KLa(C - C*) ∂t

(2)

where C* is the mobile-phase concentration in equilibrium with the stationary-phase concentration q, a is the mass-transfer area per unit volume of the bed, and KL is the overall liquid-phase mass-transfer coefficient. KLa can be called the volumetric mass-transfer coefficients in the liquid phase. The initial and boundary conditions associated with eq 1 are

At t ) 0, C ) 0 for 0 e z e L For t > 0, at z ) 0, C ) CF In the language of wave propagation theory,16 the introduction of the feed generates a self-sharpening wave. Because of the finite mass-transfer rate, the selfsharpening wave will eventually evolve into a constant pattern traveling at a constant velocity, uC. In the constant-pattern wave, the ratio of the pollutant concentrations in the stationary and mobile phases is constant:20

qF q ) C CF

(3)

where CF is the feed pollutant concentration in the mobile phase and qF is its associated equilibrium concentration in the stationary phase. Also in the constant-pattern wave, the mobile-phase concentration can be expressed as a unique function of the adjusted time defined as τ ) t - z/uC. The adsorption rate expressed in terms of the adjusted time is

F

dq ) KLa(C - C*) dτ

(4)

When q is substitiuted with qFC/CF into eq 4 and the general adsorption isotherm model of power-law type is used, q ) kCn leads to the following equation that can be used to predict the breakthrough curve:

t ) t1/2 +

[∫

FkCFn-1 KL a

x

]

1 dx x - x1/n

1/2

(5)

where x is the dimensionless effluent concentration, x ) C/CF, and t1/2 is the half-time for x ) 1/2. In eq 5 the parameter t1/2 can be directly read from the experimental data and the parameter KLa can be determined from the tangent slope of the x versus t curve at x ) 1/2:

(dxdt )

) x)0.5

KLa FkCFn-1

(x - x1/n)

(6)

Experimental Section BA with purity greater than 99.5% (Fluka Chemical Corp., Switzerland) and distilled deionized water were

Table 1. Experimental Conditions for Column Test Runs experimental condition

run 1

run 2

run 3

run 4

bed void fraction bed density (g/L bed) bed depth (cm) flow rate (cm3/h)

0.30 277.4 3 21.6

0.30 277.4 3 43.3

0.30 277.9 6 43.2

0.30 277.9 6 86.4

used to prepare the aqueous solutions for the tests in this study, and the resultant solution pH was called the natural pH. The GAC (Taipei Chemical Corp., Taiwan) was grounded and sieved with U.S. Standard screens to obtain a 24-32 mesh fraction. The sieved GAC was washed with 1 N HCl several times to remove oil and impurity and rinsed repeatedly with deionized water until the rinsed water showed the same UV absorbance intensity as that of the deionized water. Finally, the washed GAC was dried in an oven at 110 °C to constant weight before use. To determine the adsorption isotherms at natural pH and varying solution temperatures, different weights of GAC were added to the glassstoppered flasks with aqueous solutions having the same BA concentration. Then the flasks were shaken at 150 rpm and the desired temperature in a temperature-controlled shaker (Hotech, model 706) for 4 days to attain equilibrium. The BA concentrations were measured by an UV spectrometer (Milton Roy, model GENE-SYS 5) with the maximum absorbance wavelength at 225 nm and the Lambert-Beer’s constant of 13.64. The amounts of BA adsorbed onto the GAC were calculated from the mass balance relation. Various buffer solutions were used to control the solution pH in order to determine the effect of the solution pH on the adsorption isotherm at 25 °C. The column tests were carried out in a water-jacketed glass column with an inside diameter of 2.77 and a length of 60 cm. The activated carbon with known dried weight was put into the column randomly. Hot deionized water was used to wash the carbon in an upflow fashion in order to remove air bubbles and to rinse the carbon. Then, the bed density and void fraction were determined by the procedures described by Huang21 before a column test was begun. An aqueous solution with 2.46 mol/m3 BA concentration at natural pH was continuously fed to the top of the column at a desired flow rate controlled by a metering pump (Watson-Marlow, 302S/RL) until breakthrough happens. In all of the column tests, the effluent samples were intermittently collected by a fraction collector (Isco, Retriever 500) and measured by the UV spectrophotometer. The column temperature was maintained at 25 ( 1 °C, and other test conditions are summarized in Table 1. Results and Discussion At first, the adsorption isotherms of BA at natural pH and varying solution temperatures were measured and the experimental data were fitted with various isotherm models. The adsorption isotherm models, commonly found in the literature, and their parameters are listed in Table 2. As is indicated by the correlation coefficients, all of the models except the Langmuir model give good fits of the data. Furthermore, the parameters in the To´th model have clear trends: the maximum adsorption capacity qm and the dissociation constant m are independent of the solution temperature, while the adsorption equilibrium constant K1 decreases with increasing temperature. The Gibbs free energy change of the adsorption process is related to the equilibrium

Ind. Eng. Chem. Res., Vol. 40, No. 17, 2001 3777 Table 2. Effect of Temperature on the Adsorption Model Parameters for BA at Natural pH model

equation

Langmuir

q)

KCN 1 + KC

Freundlich

q)

kCn

Redlich-Peterson

q)

AC B + CM

To´th

q)

q mC

parameter

at 25 °C

at 35 °C

at 45 °C

at 55 °C

K

18.94

3.47

3.70

3.22

N R2 k n R2 A

3.22 0.94 2.92 0.27 0.99 2.98

3.22 0.98 2.31 0.37 0.98 2.62

2.99 0.98 2.16 0.33 0.96 2.73

2.67 0.95 1.87 0.35 0.99 1.90

B M R2 qm

0.01 0.79 1.00 12.5

0.10 0.77 1.00 12.5

0.19 0.90 0.98 12.5

0.01 0.67 0.99 12.5

K1 m R2

3.29 0.19 0.99

2.65 0.19 0.97

2.55 0.19 0.97

2.33 0.19 0.99

(1/K1 + Cm)1/m

Figure 1. Effect of the solution temperature on the adsorption isotherm of BA at natural pH.

constant by the following equation:

∆G ) -RT ln K1

(7)

According to thermodynamics, the Gibbs free energy change is also related to the entropy change and the heat of adsorption at constant temperature by the following equation:

∆G ) ∆H - T∆S

(8)

where R is the gas constant, T is the solution temperature, and ∆S and ∆H are the entropy change and heat of adsorption, respectively. The equilibrium constant K1 therefore varies with the solution temperature by the following equation:

K1 ) exp

(∆SR - ∆H RT )

(9)

The experimental and To´th model predicted adsorption isotherms of BA at varying temperatures are shown in Figure 1, and the linear plot of ln K1 versus 1/T is shown in Figure 2. As is shown in Figures 1 and 2, the To´th model with the equilibrium constant calculated by eq 9 fits the experimental data quite well. The entropy change and heat of adsorption calculated from the intercept and the slope are -19.9 J/mol‚K and

Figure 2. Linear plot of the adsorption equilibrium constant.

-8.8 kJ/mol, respectively. From this low value of the adsorption heat (